Chapter 2ELECTROCHEMISTRY2.1 INTRODUCTIONThe goal of this chapter is to elucidate the fundamental characteristics and tech-nological significance of electrochemical cells. A comprehensive review on thesubject is excluded since the intention hereafter is to describe the principles ofelectrochemistry, which should provide the reader with relevant key definitionsand concepts on metal reduction and metal oxidation in galvanic couplings.Thus, the principles of anodic protection and cathodic protection become un-complicated or unproblematic to understand and comprehend suitable applica-tions ofelectrochemistry for preventing localized corrosion and general corrosionon metallic structures. In general, electrochemistry deals with the chemical re-sponse of an electrode/electrolyte system to an electrical stimulation and theelectrochemical behavior of species (ions) can be assessed, including concentra-tion, kinetics, and reaction mechanisms.Electrochemical galvanic cells involve electron transfer from a metal (elec-trode) surface to a environment (electrolyte). This metal is treated as the anodedue to its ability to oxidize by losing electrons and becoming electron-deficientatoms called cations. On the other hand, the metal receiving or gaining elec-trons is the cathode since its cations in solution reduce or deposit on the cathodesurface as atoms. Therefore, an electric field must exist in the electrolyte dueto the presence of charge particles represented by ions . If an electrochemicalcell produces energy it is known as a galvanic cell and if it consumes energyit is an electrolytic cell. Nonetheless, an electrochemical process is treated asan electroanalytical technique associated with electricity and chemistry so thatelectrical quantities are measured in order to quantify chemical changes in acell. Chemical measurements normally involve heterogeneous bulk solutionsand electrochemical processes are analyzed according to the ionic interactionsat the electrode-electrolyte interface.The applications of electrochemistry is broad. Simply stated, metal ions canbe reduced into atoms on an electrode surface by chemical and electrochemical
28 CHAPTER 2. ELECTROCHEMISTRYprocesses. The former process does not involve any current flow to drive a redoxreaction, but the latter does. Eventually, metal reduction starts at a nanoscaleforming atom agglomerates or nanoparticles [13-16] and it may proceed to a mi-croscale as in thick film formation or macroscale as in electrowinning technologyfor recovering , say, cooper from solution. Nowadays, nanotechnology is gainingacceptance in the scientific community.2.2 ELECTRICAL POLESAssume that electrical conductors, such as aqueous solutions containing chargedparticles known as ions, exists in a static electrochemical system and that thereexists an infinitesimal current flow. Thus, an electric field strength vector ata point P in space and an inner electric potential of the system are definedbelow, respectively where = Electric force vector (N)Q = Electric charge (C = Coulomb)W = Electric work (J)In fact, Q depends on the type of ions, which are treated hereafter as poles,and it is related to Faraday’s constant F. Both F and Q are defined bywhere = Electron charge = (= Avogadro’s number = (= Mole fraction (mol)= Valence or oxidation numberThe Cartesian electric field strength components in a three-dimensionalscheme are defined as fallows
2.2. ELECTRICAL POLES 29where = Permittivity of vacuumMONOPOLE: Let be defined at a point P in space around a chargein an electrical monopole path shown in Figure 2.1a. Integratingeq. (2.2a) yields the inner electric potential in the x-directionEquation (2.3) gives the definition of the monopole potential due to a pointcharge Q. This is a simple definition of an internal potential between two pointslocated at a relatively short distance. Otherwise, as On theother hand, when as an electric potential “singularity” can beestablished for in the order of as predicted by eq. (2.3).Consider an electrolyte or a metal as a single electrical conductor phase inequilibrium. In this case, currentflowdoes not occur and the electric field at allpoints in the phase is zero. In fact, a non-infinitesimal current is an irreversibleprocess since heat is generated by the current flowing in the phase . Atequilibrium, eq. (2.2b)gives which means that the electricpotential is constant in the bulk phase so that and the current is I = 0.
30 CHAPTER 2. ELECTROCHEMISTRYThis can be analyzed by using eq. (2.2a) since but giveswhere C =constant; therefore, which implies that it is anet electrical charge being uniformly distributed over the surface of the phase;otherwise, the repulsive force oflike charges will not allow diffusion (motion) ofcharges to the phase surface .DIPOLE: Consider the charge couple shown in Figure 2.1b, in which thenegative and positive charges are separated by a distance makingan electrical dipole for which the electrical dipole moment has a magnitude ofSuppose that the charged particles and the point P in space make1) a right triangle Thus, an extension of the single charge casedescribed by eq. (2.3) can provide the internal electric potential Using eq.(2.3) along with yields2) If make an oblique triangle, then the electric potential isUsing the law of cosines and assuming that yieldsSubstituting eq. (e) and into (b) givesNow, letting in eq. (f) the electric potential becomes The electric potential “singularity” is in the order of sinceas Thus, the electric field strength according to eqs. (2.3) and (2.5)are, respectively
2.3. ELECTROCHEMICAL CELLS 31Notice that the E “singularity” is in the order of for the monopole andfor the dipole cases. This briefintroduction ofthe source ofthe electric fieldstrength of a phase is for the reader to notice that a phase has been treatedas an electrically neutral thermodynamic system, which is not the case for aheterogeneous electrochemical cell. In addition, this section serves the purposeof comparison with the proceeding electrochemical treatment.Example 2.1 Let an electrolyte contain a net charge due to moles ofnickel cations Calculate the surface electric potential at a distanceof 7 cm from the solid electrode-electrolyte interface in the Willthis calculated potential value differ from the electric potential differencebetween electrodes? Explain.Solution:from eq. (2.1d),But,Thus, inserting these values into eq. (2.3) gives the electric potentialThis large amount of volts does not represent a typical difference in electricpotential between electrodes of a practical electrochemical system. Normally, afew volts are needed to operate a simple electrochemical system. Conclusively,2.3 ELECTROCHEMICAL CELLSFirst of all, corrosion is basically an electrochemical process that involves ionicinteractions leading to metal dissolution or surface deterioration. Thus, the the-ory of corrosion requires thorough understanding of the electrochemical events
32 CHAPTER 2. ELECTROCHEMISTRYwithin a particular metal-electrolyte system for mitigating corrosion. This dic-tates that the driving force for electrochemical events must be known in orderto classify the type of electrochemical cells to be characterized either to recovermetals from solution (see Chapter 7) or prevent corrosion (Chapter 8).In general, electrochemical cells have four basic components calledThe electrolyte is an electrical conductive fluid or moist soil.The anode electrode is a metal in contact with the electrolyte allowinganodic reactions to take place.The cathode electrode is a metal in contact with the electrolyte allowingreduction reactions to occur on the surface.The power supply which is connected to the anode and cathode elec-trodes, providing the potential to the electrochemical system for reductionreactions (electrolysis) or current through the anode to protect the cath-ode from corrosion.Furthermore, an electrochemical system can be classified according to theschematic cells depicted in Figure 2.2. The electrochemical cells are describedbelow.1) Galvanic cell, which is a bimetallic cell since it has different metallicelectrodes, but currentflowsclockwise as indicated in Figure 2.2a by the arrows.This electrochemical event produces electric energy from the stored chemicalenergy in the metallic anode. Consequently, current flows from the cathodeto the anode through the metallic circuit and electric power , P = EI, is
2.3. ELECTROCHEMICAL CELLS 33produced. Faraday’s law of electrolysis is obeyed for forming electrochemicalreaction reactions under the principles of electrochemical stoichiometry so thatthe redox reaction occurs spontaneously without the aid of an external powersupply. The subject of electrolysis will be dealt with in Chapter 7.2) Electrolytic Cell, in which current flows clockwise as shown in Figure2.2b, but the source ofpower is external. The cell has bimetallic or mono-metallicelectrodes. This cell consumes power, P = EI, and the cell reactions are drivenin the reverse direction as opposed to galvanic ; that is, the galvanic sponta-neous reactions are driven backwards. This is possible if the applied potential isgreater than the galvanic potential. This type of cell is very useful in the elec-trometallurgy field for recovering metals from oxide ores by electroplating themetal ions on cathodes. Hence, if current flows, then the principles of electro-chemical stoichiometry is used for producing electrochemical reactions throughthe process of electrolysis and metal ions are deposited on a cathode surface.Electrolysis stands for an electrochemical process in which the redox reactionis forced (non-spontaneous) to occur by passing a direct current (dc) throughthe electrolyte. Therefore, but the measurable cellpotential difference in an electrolytic or galvanic cell can be influence by theOhm’s potential (E = IR) drop. Table 2.1 lists comparison between galvanicand electrolytic cells.3) Concentration Cell, which has mono-metallic electrodes, but the anodeis immersed in a concentrated region of the electrolyte as shown in Figure 2.2c.This cell has the electrodes made of the same metal and it is similar to a galvanicwith respect to the electrode polarity and current flow direction. The electrodesare immersed in a nonhomogeneous electrolyte, but the anode is within theconcentrated portion of the electrolyte where the concentration of species isFigure 2.3 shows two galvanic cells indicating metal dissolution at the anode(left electrode) and the direction of current flow. Figure 2.3a shows metalsand as the anode and cathode, respectively. Both are immersed in theirown sulfate-base electrolyte. Each and
34 CHAPTER 2. ELECTROCHEMISTRYconstitute what is known as anodic half-cell and cathodic half-cell, respectively.Subsequently, the electrochemical galvanic cell is composed of these two half-cells if current flows as shown in Figure 2.3a. On the other hand, Figure 2.3bshows a chemical galvanic cell due to the lack of current flow, but electron flowoccurs from the anode to the cathode through the wires.Recall that and are in their ionic state in solution(aqueous). Both metals are externally connected to a electrical circuit in orderto measure the potential difference between them. In other words, the circuitis used to measure the galvanic cell potential by a voltmeter (V). This measur-able cell potential is current/resistance dependent. If current ceases to flow, thenthe cell potential is known as the open-circuit potential or standard potential(E°), which are illustrated in Figure 2.2 for pure metal reduction. The stan-dard potential is also known as the electromotive force (emf) under equilibriumconditions: unit activity, 25°C, and 1 atm ) pressure.Figure 2.3b, on the other hand, shows an iron (Fe) galvanic cell composedof a cold worked electrode (anode) and an annealed electrode (cathode). Theformer electrode becomes the anode due to a high microstructural defects, suchas dislocation density, and internal (residual) stresses introduced during the coldworking (plastic deformation) process. The latter electrode is stress relievedduring annealing and the dislocation density is nearly zero or eliminated.The assessment of Fe-base couplings to form galvanic cells can be elucidatedusing two cases. According to the galvanic series in Figure 2.2, Fe is locatedbetween copper and zinc Suppose that a steel plate is coated withand another with Consequently, Fe is the anodefor and the cathodefor couplings. In the latter case, becomes a sacrificial anode, which isthe principle of coupling for galvanized steel sheets and pipes.
2.3. ELECTROCHEMICAL CELLS 35On the other hand, if coating breaks down, steel is then exposed to anelectrolyte and becomes the anode, and therefore, it oxidizes. These two casesare schematically shown in Figure 1.6. The cell potential of each coupling caseis determined by adding the standard potentials, but the signofand are reversed since they act as anodes. Recall that Figure2.2 illustrates standard potentials for reduction reactions. Hence,The above standard state (Table 2.2) conforms to the convention adoptedby the International Union of Pure and Applied Chemistry (IUPAC), whichrequires that all tabulated electromotive force (emf) or standard electrode po-tential values (E°) be so with respect to the standard hydrogen electrode (SHE)for reduction reactions of pure metals, such as In addition,Table 2.3 illustrates standard potentials for some compounds.
36 CHAPTER 2. ELECTROCHEMISTRYThus, atoms coat the rod or sediment to the bottom of the beaker.Eventually, this redox (overall) reaction produces chemical energy, which is dis-sipated as heat. This, then is a source of chemical energy that can be convertedto useful work by adequately designing a device called electrochemical cell asschematically shown in Figure 2.3a and 2.4. In fact, this cell is assumed tocontain charged species, but at least one electrically charged specie cannot pen-etrate all the phases of the system, and a difference in electric potential will bedeveloped between phases.
2.3. ELECTROCHEMICAL CELLS 37Furthermore, either Figure 2.3a or 2.4 can be used as the point of depar-ture for developing the thermodynamics of electrochemical systems, which isreferred to as electrochemical cells containing phases that are electrical conduc-tors, which are known as electrolytes. Thus, electrolytes are needed for theproper development of a potential difference. In a conventional electrochemicalcell set up, the cathode is the most positive electrode kept on the right handside and the anode is the most negative electrode . Thus, electronflowoccursfrom left to right through the terminals in the above Figures 2.3 and 2.4, whichare schematic representations of galvanic cells or voltaic cells.In general, an electrochemical cell can be used to drive or be driven by anexternal electrical system or device, such as an incandescent light or motor-generator, respectively. A motor-generator can drive or be driven by an elec-trochemical cell, depending on the cell potential or on the applied potential,respectively.With regard to Figure 2.4, and are contact potentials andis the liquid junction potential. The measurable standard cell potential forFigure 2.4 is a measure of interfacial potentialsIn real cases, nonstandard conditions exist and the cell potential can bepredicted bywhere and are potential terms for correcting the standardpotential expression, eq. (2.7a), These terms will be dealt with in a later section.
38 CHAPTER 2. ELECTROCHEMISTRYThe system shown in Figure 2.4 is a galvanic cell known as a voltaic cell,which consists oftwo different solids called anodic electrode and cathodicelectrode. In summary, this electrochemical coupling has several events whichcan be described as follows:1) Zinc is immersed in aqueous zinc sulfate so thatbecomes the anodic half-cell. Similarly, copper in copper sulfate,is the cathodic half –cell.2) half cell half cell.3) and are solutions known as electrolytes, which arephases like and electrodes and are electrical conductors as well.4) wire is used to connect the and electrodes so that no potentialdifference develops between the wires, which are called terminals.5) The salt bridge or porous membrane is used to connect both electrolytesand allow the migration of ions to maintain electrical neutrality of the cell.6) If a salt bridge is not used, both half-cells become isolated and electricalneutrality is lost since the electrode becomes more positive as cationsare produced and the electrode becomes more negative as are removedfrom solution and deposited as atoms on the electrode surface. Thus, thecations (positively charged particle) and sulfate anions (negativelycharged) migrate through the salt bridge in the opposite direction.7) The terminals are connected to a voltmeter to complete the well-knownelectrochemical galvanic cell circuit.8) The galvanic cell (like a battery) converts chemical energy to electricalenergy due to electronflowfrom the anode to the cathode through the terminals.9) The voltmeter is used to measure the potential difference between theand electrodes at equilibrium.2.3.1 OPEN-CIRCUIT CONDITIONThis is the case when the voltmeter is removed leaving an open-circuit. Asummary of events are outlined below for Figure 2.4.1) Due to instability of the galvanic cell, cations diffuse into thesolution through the salt bridge. Diffusion is slow, but ionswill come in contact with the electrode. Consequently, the zinc anode oxi-dizes and the copper cations reduce to form atoms as shown below. The redoxreaction results by adding both the anodic and cathodic reactions2) A spontaneous redox reaction occurs without electron flow. Eventually,the electrode will go into solution or simply dissolves.
2.3. ELECTROCHEMICAL CELLS 393) The redox reaction indicates that oxidizes in solution andreduces in solution. Eventually, the cell would be destroyed.4) In order to avoid destruction of the cell, just connect a resistor like a volt-meter to the terminals. This willkeep cations away from thesolution due to the electric field force in the solution.2.3.2 CLOSED-CIRCUIT CONDITIONThis is the case when a voltmeter (resistor) is connected to the galvanic cellfor operation purposes, so that the potential difference between the andelectrodes is measured as What happens when the cell isoperating, say, at standard condition (P = 1atm., T = 25°C, 1 mol/liter)?1) The junction potential is lower than thejunction Since electrons willflowfrom the lowestelectric potential reservoir (anodic half-cell) to the highest reservoir (cathodichalf-cell) through the external wires or terminals.2) The electrical work is for electron flow to occuras negative charges. Here, is the cell potential difference.3) If then positive chargesflowfrom low to high potential reservoirs(from to electrodes).4) Consequently, the following reactions occurThe electrons arriving at the electrolyte combine withcations in solution and deposit as atoms on the electrode surface. Thisdeposition is called electroplating.5) An electric potential difference is developed since electrolytebecomes depleted of cations and electrolyte becomes enrichedwith cations.6) Once is developed, positive ions flow through the solutionfrom to electrodes, provided that the half-cells are separated by a porousmembrane or salt bridge (Figure 2.3). According to Ohm’s Law, the change ininner potential is7) The salt bridge is filled with an agar gel (polysaccharide agar or polymergel) and concentrated aqueous salt ( or ) solution in order to maintainelectrical neutrality between the half cells (Figure 2.3). The gel allows diffusionof ions, but eliminates convective currents .8) The maximum potential difference and the corresponding cell diagram(Figure 2.5) for Figure 2.4 are given below
40 CHAPTER 2. ELECTROCHEMISTRYsinceVertical lines represent phase boundaries. A salt bridge is symbolized bytwo vertical lines and has two liquid junctions of insignificant potentials.Now that an electrochemical galvanic cell has been described in details, itis convenient at this moment to expand the thermodynamic of electrochemistryin terms of chemical energy, which in turn, will be converted to electrical en-ergy. The subsequent analytical procedure leads to the derivation of the Nernstequation, which is suitable for determining the cell electric potential when ionactivities are less than unity as nonstandard conditions.2.3.3 APPLICATION OF GALVANIC CELLSThe electrochemical galvanic cell being described so far (Figure 2.3) isa chemical energy source capable of producing 1.10 volts, which is a relativelylow energy output. This energy source capacity can be enhanced by connectingseveral cells in series. A common application of galvanic cells is in the produc-tion of batteries for flashlights, radios, automobiles and so on. For instance,the production of lead-sulfuric acid automobile batteries includelead anodes and lead oxide cathodes immersed in sulfuric acid solution. A briefdescription of these type of batteries is included in Chapter 1, section 1.4. Fur-thermore, a single galvanic cell produces 2 volts, but six (6) cellscoupled in series produce 12 volts. If the cell is coupled in parallel, the totalpotential is 2 volts, but the total current is 6 times that of a single cell. Thelifetime of these automobile batteries can be prolonged by supply-ing an external current provided by an alternator. In this case, the oxidation
2.4. THERMODYNAMICS 41and reduction reactions are reversed and the battery is maintained charged forsome time. Table 2.4 lists alloy galvanic series.2.4 THERMODYNAMICSUsing Figure 2.3a as the basic cell, the thermodynamics involved is treatedbelow in a general case. Remove the salt bridge and treat each cell as isolatedsystems. Let metal M rod be the phase being immersed in an aqueous solution(electrolyte), which is the phase Let and be the valence of thecations and the anions Let be the electric potentialof the metallic phase and the electric potential of the phase. Once thephase is in contact with the phase, an exchange of charged particles betweenand phases causes a change in the total energy of the system, which consists ofthe negatively charged phase as electrons are discharged into the electrolyte.The altered total energy is due to the change in electrostatic potential energy ofthe phases involved, specifically at the metal-electrolyte interface where a strongelectric field exists and a double layer of charged particles disturbs the charge onthe interface. This double layer is a normal balance (equal number) of positiveand negative ions, which diffuse to the interface causing such as disturbance inenergy . Eventually, the system will reach the state of equilibrium within theelectrolyte.The entropy change (dS), the electrical energy change (dE), and the changeof charge (dq) for a coupling, in which is the metallic phase and is theelectrolyte phase are, respectively
42 CHAPTER 2. ELECTROCHEMISTRYwhereUS= Chemical potential= Internal energy= Entropy= Electron charge= Electric potentialPVTF= Pressure= Volume= Temperature= Number of moles= Faraday’s constantFor an isolated thermodynamic system, the following constraints canbe used to develop equilibrium conditions and the Gibbs free energy changeHence, combining eq. (e) and (2.14) and the resultant expression with eq.(a) yieldsThe physical interpretation of these constraints, eqs. (f) and (g), and eq.(2.14) implies that adding and moles to the phase and thephase, respectively, the change in electron charges becomes Substituting eqs. (a) and (f) into (2.14) and (2.14) into (2.13) yields
2.4. THERMODYNAMICS 43Substituting eqs.(a) through (k) into (2.11) and (2.12) and the resultantexpressions into (2.10), and subsequently, collecting terms yields the entropychange of the systemAt equilibrium, dS = 0 and the following is deduced from eq. (2.15) 1) For thermal equilibrium,2) For mechanical equilibrium,3) For electrochemical equilibrium, andThus, is the affinity forand is the Gibbs free energy change for the system.In addition, the potential difference between two phases in a half-cell at equilibrium cannot be measured. Instead, two electrodes are connectedas shown in Figure 2.3a to measure the electric potential difference between theelectrodes. This can be done by connecting, say, system to the previoussystem using a salt bridge or porous membrane. Thus, the electric potentialdifference between the and electrodes is Recall that thesalt bridge is a glass tube filled with an electrolyte that allows charge transferbetween the cell electrolytes without disturbing the equilibrium state.
44 CHAPTER 2. ELECTROCHEMISTRYApply the generalized expression given by eq. (2.19) to the galvanic cellshown in Figure 2.3a. Thus, the anodic and cathodic reactions and their re-spective energy change expressions are, respectivelyIn order to balance the number ofelectrons in eqs. (2.21) and (2.22), multiplyeq. (2.21), as well as eq. (a), by and add them up to get the redox reactionand its energy change aswhereIn general, the equilibrium and no-equilibrium energy change expressionsare, respectivelyUsing the argument for deriving eq. (2.19), the standard Gibbs free energychange can be defined in a general form aswhere = Number of ions or molecules in an reaction= Specie involved in the reactionCombining eqs. (2.26) and (2.27) yields the standard electric potential interms of standard chemical potential
2.4. THERMODYNAMICS 45Table 2.5 illustrates standard chemical potentials for some metals, ions, andmolecules. A more complete data can be found in Pourbaix work [18-19]. Ap-plying eq. (2.28) to the redox reaction given eq. (2.23) yieldsExample 2.2 Let’s apply the above generalized procedure to the galvaniccell shown in Figure 2.4. Assume that the cell is in equilibrium and that thecell phases are with withand Will the redox reaction occur?Solution:Using eqs. (2.23) and (2.24) along with(Figure 2.4) and yieldsTherefore, the redox reaction occurs spontaneously as written sinceExample 2.3 Let the anodic phases be with andwhereas the cathodic phases are with
46 CHAPTER 2. ELECTROCHEMISTRYand a) Determine the redox reaction using eq. (2.23) and b)calculate the Gibbs free energy change. Will the redox reaction occur?Solution:a) From, eq. (2.23),b) According to Figure 2.3a, the cell potential isand from eq. (2.24), the standard free energy change isTherefore, the redox reaction occurs spontaneously as written sinceExample 2.4 Use the data given in Table 2.5 to determine the half-cells andthe redox standard potentials for the galvanic cell shown in Figure 2.4. Comparethe results with the data given in Table 2.2.Solution:From eq. (2.28) and Table 2.5,
2.4. THERMODYNAMICS 47These results are exactly the same as given in Table 2.2. Thus, eq. (2.7b)yields the standard cell potentialIn addition, the activity of a specie for a redox reaction can be deter-mined by considering the change in free energyFor an isothermal (T = constant) and isometric system, eq.(2.29) yieldsorwhere PRT= Pressure= Standard pressure = 1 atm,= (Universal gas constant)= Absolute temperature (°K)Thus, the activity is defined asAt standard conditions, T = 25°C, andTable 2.6 illustrates some important definitions, which are needed to solve elec-trochemical problems.
48 CHAPTER 2. ELECTROCHEMISTRYNow, the equilibrium constant K for eq. (2.23) can be defined in terms ofactivities as follows:Using eqs. (2.29a) and (2.30a) for a redox reaction yieldsSolving eq. (2.30c) for the no-equilibrium energy change givesAt standard conditions, and eq. (2.31a) becomesThus, the equilibrium constant K can be determined from measurements ofthe electric potential or chemical potentialSubstituting eqs. (2.25) and (2.26) into (2.31a) yields the Nernst Equationfor calculating the nonequilibrium electric potential (E) of an electrochemicalcell. Hence,The interpretation of the Nernst equation suggests that the current result-ing from the change of oxidation state of the metals and is known
2.4. THERMODYNAMICS 49as Faradaic current, which is a measure of the rate of redox reaction. Theterm in eq. (2.32) stands for the number of coulombs needed for reacting1 mol of an electroactive specie. Therefore, eq. (2.32) embodies the Faraday’slaw of electrolysis since the redox reaction involves electron transfer betweenphases having different electric potential. For instance, electrochemical equi-librium is achieved if current flow ceases in a reversible galvanic cell (Figure2.3). Despite that the Nernst equation is derived assuming thermodynamicequilibrium of a reversible cell, K in eq. (2.32) is not exactly the same as thechemical equilibrium constant due to a current flow. The Nernst equation givesthe open-circuit potential difference (emf) for a reversible galvanic cell and ex-cludes liquid junction potentials [see eq. (2.7a)], which are always present, butsmall in magnitude. For example, the liquidjunction potential difference for thecell in Figure 2.4 is but it is not completelyeliminated after a salt bridge is connected.From a macroscale, the Nernst equation is graphically depicted in Figure2.6, which elucidates a simple calculus plot. The intercept is just the standardpotential (E°) at 25°C and the slope, is the energy/charge ratio.Example 2.5 Apply the preceding procedure to the galvanic cell shownin Figure 2.4 or to the cell diagram in Figure 2.5 at a temperature of 25°Cfor determining a simplified expression for the equilibrium constant K and theNernst cell potential E.Solution:From eq. (2.30b),since (solids) = a (molecules) = 1 mol/liter. Thus, the cellpotential defined by eq. (2.32) along with and(Figure 2.4) becomes
50 CHAPTER 2. ELECTROCHEMISTRYExample 2.6 Derive the Nernst equation, eq. (2.32), using the anodic andcathodic reactions for Figure 2.4.Solution:Then,Example 2.7 The application of eq. (2.32) is suitable for determining theactivity of ions when the anodic half-cell is mechanicallykept replenished so that If current ceases to flow inthe galvanic cell shown in Figure 2-4, calculate the activity and the concentrationof copper ions in at 25°C.Solution:From eq. (2.32) and Example 2.5,
2.4. THERMODYNAMICS 51Solving for yieldsFrom Table 2.6, the concentration of iswhich is very low.An electrochemical cell can be used to measure the entropy change andthe enthalpy change of a reversible reaction. This can be accomplishedby measurements of the Nernst potential (E) as a function of temperature. Atconstant pressure, the free energy change and are defined byDifferentiating eq. (2.26) with respect to the temperature T yieldsThen, the entropy change becomesThe reversible thermal energy (heat) is defined bySubstituting eqs. (2.33) and (2.26) into (2.34) yieldsThe heat capacity at constant pressure (P) is defined byFrom eq. (2.35),
52 CHAPTER 2. ELECTROCHEMISTRYUsing an electrochemical cell to measure the cell potential, eq. (2.32), as afunction of temperature at constant pressure leads to curve fitting an empiricalfunction, usually a polynomial. One particular polynomial is of the form where = Reference temperature (K)a, b, c, d = Curve fitting coefficientsNow, the above thermodynamic state functions can be defined in terms oftemperature. Thus,Example 2.8 Levine  applied eq. (2.40) as continuous function in theclosed temperature interval [0ºC, 90ºC] or [273.15 K, 363.15 K] for plating sil-ver (Ag) from silver chloride (AgCl) according to the following redox (overall)reactionThe curve fitting coefficients at P = 1 atm and areCalculate a) and at T = 25 °C and b) usethe Rolle’s theorem to determine if the functions E = f (T) and aredifferentiable in the open temperature interval [273.15 K, 363.15K].Solution:
2.5. STANDARD ELECTRIC POTENTIAL 53a) If T = 25 °C = 298.15 K, and F = 96,500 C /mol= 96,500 J /mol V, then the following resultsFrom eq. (2.40),From eq. (2.43),From eq. (2.44),From eq. (2.37),From eq. (2.86),From eq. (2.45),These results indicate that can be plated at T = 25 °C sinceand Notice that the calculated valuefor matches with the value given in Table 2.3.b) The required plots, E = f (T) and are shown below as per eq.(2.40) and (2.43), respectively. According to Rolle’s theorem the derivatives areand and, E = 0.252V and atT = 211.84 K. The condition E(a) = E (b) and aremetintheopen interval [273.15 K, 363.15 K]. For instance, E(100) = E (343.36) = 0.19V and Therefore, bothfunctionsare continuous and differentiable.2.5 STANDARD ELECTRIC POTENTIALIn this section, a procedure to carry out measurements of the electromotive force(emf) is described. This emf is known as the standard potential alreadyintroduced in Table 2.2. The standard hydrogen electrode (SHE) is used as thereference electrode in conducting these measurements. In general, a referenceelectrode one selects tomeasure of a metal has to be reversible since classical
54 CHAPTER 2. ELECTROCHEMISTRYthermodynamics applies to all reversible processes. The SHE cell diagram forthe potential measurement is shown in Figure 2.7 and the schematic cell isshown in Figure 2.8.Nonetheless, the SHE is a gas electrode that consists of a platinum foilsuspended in sulfuric acid solution having unit activity at1 atm and 25 °C. In order to maintain mol/l purified hydrogengas is injected into the anodic half-cell in order to remove any dissolved oxygen.The platinum foil is an inert material in this solution and it allows the hydrogenmolecules to oxidize, providing the electrons needed by the metal ions tobe reduced on the cathode surface. The concentration of ions are also keptat unit activity. By convention, the standard hydrogen electrode potential iszero;In addition, Table 2.7 lists some conversion of potential vs. SHE and half-cell reactions for secondary reference electrodes used for measuring corrosionpotentials of metals and alloys in specific applications.
2.5. STANDARD ELECTRIC POTENTIAL 55Example 2.9 If the potential of a metal M with respect to the saturatedcolomel electrode (SCE) is -0.541 V, convert this measured potential to SHEpotential.Solution:If E = –0.541 thenE = (–0.541 + 0.241)As can be seen in Figure 2.8, the metal M is coupled with theplatinumelectrode and the electric potential of M at the surface is measured against theSHE. Recall that this potential is the resultant of several interfacial potentialsdescribed by eq. (2.7a). The junction potentials of the and M electrodesare small, equal, and apposite so that they cancel out. The liquid junctionpotential is also small and negligible. The cell potential is also known as theinterfacial cell potential, which depends on the chemical potential of thespecies (ions) in solution at equilibrium and it is predicted by eq. (2.28). Theelectrons flow toward the cathodic electrode M, where the metal cationsgain these electrons and enter the electrode lattice. This is a reduction processthat strongly depends on the chemical potential of the cations.The spontaneous redox reaction in Figure 2.8 isand the standard cell potential using Table 2.5 isFor instance, if thenThis is exactly the result given in Table 2.2.
56 CHAPTER 2. ELECTROCHEMISTRY2.6 POURBAIX DIAGRAMSPotential-pH plots are known as Pourbaix diagrams since they were first madeby Pourbaix in 1938. A compilation of these diagrams is available in the Atlasof Electrochemical Equilibria in Aqueous Solutions . In practice, Pourbaixdiagrams are suitable for studies of corrosion, electrowinning, electroplating,hydrometallurgy, electrolysis, electrical cells, and water treatment since theyare electrochemical maps indicating the domain of stability of ions, oxides andhydroxides . Thismapprovides theoxidizingpower inanelectrochemical fieldmeasured as potential and the acidity and alkalinity of species measured as pH.Thus, any reaction involvinghydroxyl should be written in termsof concentration, which in turn is converted into pH. The conversionfactor is given in Table 2.6. Besides the possible reactions that may occur inan electrochemical system, a simplified Pourbaix diagram gives important areasfor designing and analyzing electrochemical systems. These areas are known ascorrosion, passivation, and immunity. However, a Pourbaix diagram does notinclude corrosion rate, which is essential in kinetic studies.2.6.1 DIAGRAM FOR WATER AND OXYGENThe construction ofthe E-pH Pourbaix diagram for water and oxygen is straight-forward. Consider the hydrogen evolution reaction at standard conditions (T =25°C,for which the equilibrium constant isFrom eq. (2.32), the Nernst equation gives the hydrogen potential aswhere b = slope = –2.303RT/F = –0.0592V, Z = 2, andFigure 2.9 shows the plot for eq. (2.47) labeled
2.6. POURBAIX DIAGRAMS 57For oxygen in an acid solution,whereUsing eq. (2.32) along with Z = 4 yieldsPlotting eq. (2.48) yields a straight line as shown in Figure 2.9. Notice thatthe slope does not change if and change. Usually, thesestraight lines are superimposed on a metal diagram for comparisonpurposes.Analysis of Figure 2.9:@ water is unstable and decomposes to hydrogen gasThus,@ atm, eq. (2.47) becomes and establishes thelimit of predominance between and but predominates.
58 CHAPTER 2. ELECTROCHEMISTRY@ water is stable@ water is stable@ eq. (2.48) becomes and itestablishes the limit of predominance between and but predomi-nates.@ predominates.Example 2.10 Drive eq. (2.48) for an alkaline solution and compute theand for a pH = 10 under standard conditions.Solution:from whichFrom Table 2.6,Then, eq. (c) becomesFrom eq. (2.32) with and Z = 4,becomesIt can be concluded that eq. (2.48) gives the same result if either acid oralkaline solution is selected.
2.6. POURBAIX DIAGRAMS 592.6.2 POURBAIX DIAGRAM FOR A METAL MBelow is a brief description on how to construct a Pourbaix diagram for a metalelectrochemical system. Figure 2.10 shows a schematic and yet, sim-ple Pourbaix diagram, which includes the water and oxygen lines forcomparison purposes. The construction of the diagram consists of determiningthe potential E for lines 1 and 3 using the Nernst equation, and the pH for lines2 and 4 using known equilibrium constant K. The range of metal ion concen-tration can be butis chosen hereafter in order to simplify the procedure for constructing the di-agram. Otherwise, several vertical and incline lines would be generated. Ifthe electrochemical corrosion process is unrealistic . Theprocedure is as follows1) Horizontal Line 1:This reaction involves electron transfer only. Thus, the Nernst equation, eq.(2.32), with and T = 298K becomes
60 CHAPTER 2. ELECTROCHEMISTRYThe value for the standard potential is given in Table 2.2, providedthat the metal M is known. Thus, eq. (2.49) plots a horizontal line shown inFigure 2.10 as line 1.2) Vertical Line 2:This reaction involves a fixed hydrogen concentration only, the equilibriumconstant K for this reaction must be known so thatTherefore, a straight line is drawn starting at point. This is shownin Figure 2.10 as line 2. It should be mentioned that the metal oxidecan be replaced by a metal hydroxide or depending on thechosen metal. Thus, eq. (2.50) should be balanced accordingly. Hence,3) Incline Line 3:Notice that this reaction involves both hydrogen and electron transfer. Then,the Nernst equation becomesThe standard potential must be known. In Figure 2.10, Line 2 andline 3 intersect at a pH value given by eq. (2.51). Above this pH, a passivationprocess takes place on the metal surface according to the following reactionwhere is a passive film compound. This reaction is reversed belowthe pH given by eq. (2.52).4) Vertical Line 4:
2.7. ELECTRICAL DOUBLE LAYER 61Letting in eq. (a) yieldsSolving for givesSubsequently, a vertical line 4 is drawn at this value.2.7 ELECTRICAL DOUBLE LAYERWhen a metal M is immersed in a suitable electrolyte, initially its atoms oxidizeat a relatively high rate, and subsequently, the oxidation (dissolution) processgradually ceases and eventually stops due to a negative charge build-up onthe metal surface. Thus, the dynamic equilibrium is attained, provided thatno other complex electrochemical reactions take place. In this process, metalatoms are removed from their lattice sites to ionize as cations into theelectrolyte, forming a negatively charge metal surface. If polar watermolecules and hydrogen cations are in the electrolyte, they are attractedby the negatively charged metal surface to form an ionic structure (layer), whichprevent other ions from the bulk solution to be part of it. This structure isa complex ionic arrangement in an electric field and has a limited thickness.Eventually, metal dissolution ceases if there is no external current flow, but itproceeds until the ionic structure is dense enough to protect and prevent themetal from reacting any further until equilibrium is reached. With respect tothe the metal-layer-bulk within which there must exists an electric potentialdecay. The ionic structure is known in the literature as the electrical double-layer (EDL). This EDL seems to limit the continuous electrochemical reactionsat the metal surface due to the lack of charge transfer.One finds in the literature [10-12] different models for explaining the inter-facial structure of the electrical double layer. This layer is referred to as theHelmholtz layer which behaves like a charged capacitor. Figure 2.11 shows anschematic electrical double-layer model.
This model indicates that some negatively charge ions are adsorbed on themetal electrode surface and polar water covers the rest of this surface, form-ing a protective layer. The positively charged hydrogen is in contact with thenegatively charge metal surface. Thus, one can conclude that1) The Inner Helmholtz Plane (IHP) is an ionic layer that consists ofadsorbed dipole molecules. The majority of the anions do not penetratethis layer, some do as indicated in Figure 2.11. The inner potential on theboundary of this ionic plane is2) The Outer Helmholtz Plane (OHP) consists of a plane of adsorbedions due to electrostatic forces in contact with a diffuse ionic layer at a innerpotential3) The Diffuse Layer (DL) is a thick layer located in a region of diffuselyions in contact with the OHP and the bulk of solution at a potential range ofThus, the diffuse layer/bulk boundary is atThe distribution of the inner electric potential in solution is shown inFigure 2.12 and defined by where = constant and = distance from the metal surface.In fact, this mathematical model represents an electric potential decay since62 CHAPTER 2. ELECTROCHEMISTRY
The concentration of the oxidized species, may be predicted using theNernst equation, eq. (2.32). In this case, the potential E is replacedby Thus,for a species the interfacial potential within the electrolyte is defined bywhere K =K = Rate constant= Concentration (activity) at= Concentration (activity) atSolving eq. (2.59) for yields the concentration decay function, whichis dependent on both interfacial potential and temperature TFor small values of eq. (2.60) can be linearized by expanding theexponential function using Taylor’s series. Hence,The resultant expression implies that there is a linear relationship betweenand2.7. ELECTRICAL DOUBLE LAYER 63
2.8 DEGREE OF DISSOCIATIONSince electrolytes transport charge in the solid, aqueous or vapor state, it isworthwhile mentioning that the degree of dissociation of a compound added toa solvent can be estimated by the degree of dissociation parameter Elec-trolytes hereafter are treated as aqueous electrolytes (solutions) unless otherwisestated. In general, if the solution is a weak electrolyte and ifthe solution is a strong electrolyte since the compound being added to a solventcompletely dissociates into ionic components, such as cations and anions.Consider the following reaction for a salt dissolved in a solventwhere M is a metal and O is an oxide or hydroxide. The ionic componentsare metal cations and oxide or hydroxide anions.The standard free energy change for chemical equilibrium and the equilib-rium constant are, respectivelyThe activity or molar concentration the degree of dissociation andthe total molar activity are define as follows Substituting eq. (2.64) into (2.63) yieldsIf then eq. (2.65) becomesfrom whichThis expression indicates that the degree of dissociation increases with in-creasing concentration; that is, as Further, if a hydroxylion activity is related to a hydrogen ion activity through the dis-sociation of water. Hence, the dissociation constant for water is64 CHAPTER 2. ELECTROCHEMISTRY
For a neutral solution, Also, the acidity or alkalinityof a solution is defined by the pHHence,This hydroxyl concentration may be used in the dissociation of a metalhydroxide compound, such as An example can make this procedurevery clear.Example 2.11 Determine the amount of silver hydroxide neededto make one liter of silver-containing electrolyte having a pH = 11.6 at 25°Cand 1 atm. The dissociation constant of is The atomicweight of silver is 107.87 g/mol and the molecular weight of is 124.87g/mol.Solution:In this problem, the silver hydroxide is assumed to dissolve to an extent inpure water. The reactions of interest areandFrom eq. (2.70) and 2.71),2.8. DEGREE OF DISSOCIATION 65
From eq. (2.66) with the total silver concentration in solution ispredicted bySolving for in eq. (c) yieldsFrom eq. (2.64b),Substituting eq. into givesFrom eq.which implies that the solution is a weak electrolyte since The totalweight of added to water solvent isTherefore, add 17.98 grams of solid to one liter of pure water,stir until a homogeneous electrolyte is attained. This electrolyte can be used forsilver plating purposes.66 CHAPTER 2. ELECTROCHEMISTRY
2.9 SUMMARYIt has been shown that the potential difference of an electrochemical galvaniccell is where both and are the inner surface potentials andthe sum of the junction potentials was assumed to be very small. Thus, therepulsive forces of like charged particles (ions) in an electrical polypole systemallow diffusion of these particles to the phase surfaces. This is a significantelectrochemical process to convert chemical energy into electrical energy as inthe case of a battery flash light. In principle, electrical energy can be convertedinto chemical energy as in the case of electrolysis of copper ion reduction wherethe cell potential isIn addition, can be predicted by the Nernst equation, eq.(2.32). If the standard hydrogen electrode (SHE) is coupled with a pure metalelectrode, the standard metal electrode potential issince Moreover, the inner surface potential is where isthe distance from the metal electrode surface. It is assumed that decayslinearly through the Helmholtz double layer and exponentially inthe diffuse layer and bulkAn electrochemical cell can be used to determine thermodynamic energychanges like the change in entropy change in enthalpy change inGibbs freeenergy the heat capacity at constant pressure and thereversible thermal energy (heat) Q.Also, Pourbaix diagrams being electrochemical maps of ionic species canbe constructed using electrochemical cells containing water as the solvent at aconstant temperature. These diagrams are potential-pH plots that show areasknown as corrosion, passivation, and immunity. In spite of the usefulness ofthese diagrams for characterizing electrochemical systems, kinetics parameters,such as corrosion rate, cannot be predicted from such diagrams.Electrolytes can be classified as strong or weak solutions through the degreeof dissociation parameter Thus, if then the electrolyte is weak;otherwise, strong if2.9. SUMMARY 67
2.10 PROBLEMS/QUESTIONS2.1 Define the galvanic electrode potential for the cell shown in Figure 2.4using the interfacial potentials involved in the electrochemical process.2.2 Described what happens in the galvanic cell shown in Figure 2.4 whenelectrons leave the Cu terminal at the Cu-Zn interface.2.3 Explain why an electrode potential difference occurs in Figure 18.104.22.168 Why are cations electroplated on the electrode surface inFigure2.4?2.5 Calculate the standard potential for the formation of ferric hydroxide(brown rust).2.6 Consider the following electrochemical cell tocalculate the maximum activity ofcopperions in solution due to oxidationof a copper strip immersed in sulfuric acid at 25°C, 101 and[Solution:2.7 Consider a galvanic cellCalculate the cell potential using the Nernst equation at 25 °C. [Solution;2.8 The dissociation of silver hydroxide, is at 25°C inan aqueous solution. a) Derive an expression for the degree of dissociation as afunction of total activity and plot the resultant expression forb) calculate the degree of dissociation constant when the molarconcentration is and c) determine the Gibbs free energychange [Solutions: b)2.9 Calculate a) the concentration of and at 25 °C and b)the pH if and [Solutions: a)and b)2.10 If an electrochemical copper reduction reaction at 25 °C and 101 kPaoccurs at an infinitely low current density calculate a) the Gibbs free energychange as the driving force, b) the equilibrium constant K and c) thecopper ion concentration in [Solutions: a) b)c)2.11 Use the electrochemical cellto calculate a) the temperature for an electric potential of 0.762 and b)and Q. [Solutions: a) and b)68 CHAPTER 2. ELECTROCHEMISTRY
2.12 Pure copper and pure cobalt electrodes are separately immersed insolutions of their respective divalent ions, making up a galvanic cell that yieldsa cell potential of 0.65 Calculate a) the cobalt activity if the activityof copper ions is 0.85 mol/l at 25 °C and b) the change in entropy andGibbs freeenergy [Solutions: a) and b)and2.13 Show that the activities are in a galvanic cell, pro-vided that the potentials is2.14 Show that ln K in a galvanic cell at constant pressure.2.15 Derive an expression for ln for the given cells below.Assume that the current ceases to flow and that the cells are not replenishedwith fresh solutions. Plot the expressions for a temperature range ofand draw some suitable conclusions to explain the electrochemicalbehavior based on the resultant trend. [Solutions: a)and b)2.16 Explain why care must be exercised in using the galvanic series illus-trated in Table 2.2?2.17 If zinc and copper rods are placed in salt water, a direct chemicalreaction may slightly corrode zinc. Why?2.18 Is the cell potential a surface potential? If so, why?2.19 Prove eq. (2.59).2.20 Assume a solution containing a concentrations ofand at 25°C. Determine the concentration of copper ions forhydrogen evolution to occur. [Solution:2.10. PROBLEMS/QUESTIONS 69
2.11 REFERENCES I.N. Levine, “ Physical Chemistry,” McGraw-Hill Book Company, New York,(1978) 350-396. D.L. Reger, S.R. Goode, and E.E. Mercer, “ Chemistry: Principles &Practice,” Second Ed., Saunders College Publishing, New York, (1997) 795. R.T. Dehoff, “Thermodynamics in Materials Science,” McGraw-HillInc., New York, (1993) 458-484. J.W. Evans and L.C. De Jonghe, “The Production of Inorganic Mate-rials” Macmillan Publishing Company, New York, (1991) 1497-149. D.A. Jones, “Principles and Prevention of Corrosion,” Macmillan Pub-lishing Company, New York, (1992) 39-70. G.F. Carter, “Principles of Physical and Chemical Metallurgy” Ameri-can Society For Metals. Metals Park, Ohio 44073, (1979) 316-317. A.L. Rouff, “Materials Science,” Prentice-Hall Inc., New Jersey, (1973)697. D.L. Piron, “Potential versus pH (Pourbaix) Diagrams,” in CorrosionVol. 13, American Society For Metals, ASM Handbook, ninth edition, MetalsPark, Ohio 44073, (1987). M. Pourbaix, “Atlas of Electrochemical Equilibria in Aqueous Solu-tions,” NACE, Houston, Texas, (1974). J. O’M Bockris, et al., Proc. Roy. Soc. A274 (1963) 55. C.A. Barlow, Jr., “The Electrical Double Layer,” in Physical Chemistry:An Advanced Treatise, Vol. IXA/Electrochemistry, Edited by Henry Eyring,Academic Press, New York, (1970). T. Erdey-Gruz, “Kinetics of Electrode Processes,” Wiley-Interscience,John Wiley & Sons Inc., New York, (1972) 442. A. Corrias et al., Chem. Mater., 2 (1990) 363. J. Yiping et al., J. Appl. Phys., 69 (1991). G.N. Glavee et al., Inorg. Chem., 32 (1993) 474. K. J. Klabunde and C. Mohs, in “Chemistry of advanced Materials:an overview, ” Ed. by L.V. Interrante and M.J. Hampden-Smith, Wiley-VCH,New York, (1998) 271-316. P.T. Taney, Jean-Remi Butruille, and T.J. Pinnvaia, in “Chemistry ofadvanced Materials: an overview, ” Ed. by L.V. Interrante and M.J. Hampden-Smith, Wiley-VCH, New York, (1998) 329-379. M. Pourbaix, “Enthalpies Libres de Formations Standards, ” CebelcorReport Technique, 87 (1960). “Corrosion” Vol. 2, Corrosion Control, Edited by L.L. Sheir, R.A.Jarman, and G.T. Burstein, Butterworth-Heinemann, Boston, (1994) 21:12-21:24. O.C. Mudd, Corrosion, Vol. 1, 1 (1945) 192-201.70 CHAPTER 2. ELECTROCHEMISTRY